Kinetics of Recovery of Alumina from Aluminium Casting Waste through Fusion with Sodium Hydroxide
1Department of Materials and Metallurgical Engineering, Bangladesh University of Engineering and Technology, Dhaka, Bangladesh
2Bangladesh Council for Scientific and Industrial Research, Dhaka, Bangladesh
Aluminium dross containing 72% Al2O3 and 14.0% SiO2 was fused with NaOH for a period of up to 60 minutes in the temperature range of 500 – 750°C in a stainless steel crucible. The fused mass was dissolved in water. Amount of alumina in the solution was determined by EDTA compleximetric (masking and demasking) chemical method. The optimum condition for alumina extraction was determined as NaOH to aluminium dross weight ratio = 3.5, temperature = 750°C and time 60 minutes. Avrami-Erofeev equation [-ln (1-α) = (k3t) m, m = 3/2] seemed to be most appropriate one to fit the kinetic data of fusion of aluminium dross with NaOH. The activation energy was found to be 6.452kJ/mol.
At a glance: Figures
Keywords: alumina recovery, aluminum foundry waste, sodium hydroxide, fusion, reaction mechanism, kinetics, activation energy
American Journal of Materials Engineering and Technology, 2013 1 (3),
Received December 28, 2012; Revised May 29, 2013; Accepted May 30, 2013Copyright: © 2013 Science and Education Publishing. All Rights Reserved.
Cite this article:
- Sultana, U K, et al. "Kinetics of Recovery of Alumina from Aluminium Casting Waste through Fusion with Sodium Hydroxide." American Journal of Materials Engineering and Technology 1.3 (2013): 30-34.
- Sultana, U. K. , Gulshan, F. , Gafur, M. A. , & Kurny, A. S. W. (2013). Kinetics of Recovery of Alumina from Aluminium Casting Waste through Fusion with Sodium Hydroxide. American Journal of Materials Engineering and Technology, 1(3), 30-34.
- Sultana, U K, Fahmida Gulshan, M A Gafur, and A S W Kurny. "Kinetics of Recovery of Alumina from Aluminium Casting Waste through Fusion with Sodium Hydroxide." American Journal of Materials Engineering and Technology 1, no. 3 (2013): 30-34.
|Import into BibTeX||Import into EndNote||Import into RefMan||Import into RefWorks|
Dross is generated during melting of aluminium. Typically 15-25 kg of dross is produced per metric ton of molten aluminium . The main constituent of dross is aluminium, which varies from 8-80% depending upon grades. Apart from aluminium metal, dross may also contain other chemical compounds e.g. MgF2, SiO2 and MgO etc . A number of investigations have been carried out to extract alumina from different types of secondary sources such as micas, anorthite, spent catalysts [3, 4], clays and kaolins [5, 6], fly ash  etc. Attempts have been made to extract alumina from the secondary sources by adopting either pyro- or hydrometallurgical methods [8, 9]. All these secondary sources have the potentials to be the industrial raw material as they are rich in alumina content.
Amer carried out the dissolution of waste dross in sulphuric acid in order to produce highly pure aluminum sulfate . However, the process has found little practical application because of the environmental hazard due to the highly corrosive nature of the concentrated acid and alkali involved. Miskufova et al studied the leachability of aluminium from aluminium dross fines in alkaline solution at atmospheric condition . He found a maximum extraction of about 42 % of total Aluminium content by leaching of dross fines in 10 % NaOH solution.
Beaulieu et al developed a process for preparing aluminium chloride by (i) leaching aluminium dross residues with HCl, (ii) hydrochlorinating the liquid to form a precipitate comprising aluminium chloride and (iii) converting aluminium chloride into alumina .
Lucheva et al  described a process - similar to Bayer’s process - for recovery of Al(OH)3 from black aluminium dross. They leached dross in 10% NaOH solution at ambient temperature for 2 hours and precipitated Al(OH)3 by bubbling CO2 through the leach liquor. Park et al also noted that alkaline leaching of aluminium dross followed by precipitation of aluminium hydroxide Al(OH)3 is a potential method for the recovery of alumina from dross . This method of fine aluminium dross processing is economically and environmentally convenient. However, dross is a very heterogeneous material and applicability and efficiency of proposed method for individual dross samples should be experimentally investigated
In this study, aluminium dross was fused with caustic soda so that sodium aluminate can be formed. This sodium aluminate is useful for the determination of alumina in dross and also for the recovery of alumina. Maximum formation of sodium aluminate is facilitated by a high temperature of fusion.
2. Experimental2.1. Material Composition
The compositional analysis of the aluminium dross was done by the x-ray fluorescence analysis and the x-ray diffraction analysis was performed to find out the phases present in it. The result of the analysis is shown in the table below:
Figure 1 shows an X-rays diffraction pattern of the fine aluminum dross samples. Almost all of the peaks are identified. Some very small peaks could not be identified. All phases are mentioned in the Table 2.
Dross of different weight was mixed with a specified amount of sodium hydroxide (NaOH). The mixture was put in a stainless steel crucible, covered with a cap and placed in a muffle furnace. The fused sample was cooled to room temperature and dissolved in distilled water. The solution was filtered and the amount of alumina in the solution was determined by EDTA compleximetric (masking and demasking) chemical method. The effects of NaOH to aluminium dross ratio in the range 2.0-4.0, temperature in the range 500 – 750°C and time of fusion of up to 60 minutes on the extent of alumina recovery were studied. The activation energy of fusion was determined and a kinetic model was fitted for the fusion process.
3. Results and Discussion3.1. Compositional Analysis
From Table 1 it can be seen that the alumina constitutes the major portion of the sample and silica is the second major constituent.3.2. Phase Analysis
Most of the major peaks in the x-ray diffraction pattern correspond to alumina and silica. This is in good agreement with the results of compositional analysis.3.3. Optimisation of Fusion Parameters
3.3.1. Optimization of NaOH to Aluminium Dross Ratio
Effect of sodium hydroxide (NaOH) to aluminium dross ratio (weight basis) in the range 2.0-4.0 was studied. The extraction of alumina was found to increase with an increase in concentration of sodium hydroxide in the fusion mixture up to a sodium hydroxide to dross ratio of 3.5 (Figure 2). This ratio sodium hydroxide to dross was taken to be the optimum and was kept constant in the subsequent experiments.
3.3.2. Optimization of Temperature
Figure 3 shows the extent of extraction increased with an increase in reaction temperature up to 750°C.
These experiments were conducted at a constant NaOH to dross weight ratio of 3.5 and for a time period of 1h. It can be said that the dross and sodium hydroxide mixture fused at 750°C showing the maximum yield.
3.3.3. Optimization of Time
To optimize the time of fusion NaOH-dross mixture was fused for different periods of time by using the optimized parameters of fusion (temperature= 750°C, NaOH/dross ratio = 3.5). It was found that maximum yield was obtained after 60 minutes (Figure 4).
In systems involving solid reactants, the chemical reaction takes place at the interface of the reactants to produce a final compound . Diffusion must then occur through the product for the reaction to continue and the chemical reaction will proceed at the interface of one or both of the reactants. The mechanisms of these steps depend upon the experimental conditions and upon the characteristics of the solid reactants; therefore, the overall rate of the process may be controlled by chemical kinetics or transport processes.
The following Kinetic Models are usually considered for the study of such reactions 
1.Ginstling and Brounshtein: 1-2/3α-(1-α) ^ (2/3) = k1t
2.Jander equation : [1-(1-α)^(1/3)]^2=k2t
3.Avrami-Erofeev equation: -LN (1-α) = (k3t)m
α= fraction of reacted particles
t = time for fraction of reacted particles
ki = specific rate constant
m= parameter which depends on geometry
From Figure 5 time required for different fractions of reacted particle of alumina were calculated at 500°C, 600°C and 750°C and then plotted according to equation (1) to equation (3) in Figure 6 to Figure 9. Correlation of coefficient values of the plotted lines are also shown in these figures. It can be seen that the correlation is not high enough for all temperatures and also the lines do not pass through the zero point. Figure 6 suggests that the dissolution of alumina in dross is not follow the Ginstling and Brounshtein equation. Figure 7 suggests that the dissolution does not follow the Jander mechanism. So none of these two mechanisms are suitable for explaining the kinetics of the fusion procedure.
In order to investigate if the mechanism represented by Avrami-Erofeev equation i.e. -ln (1-α) = (k3t)m is the mechanism, the left hand side of Equation (3) for m=1, 2 and 3 were plotted against time for different temperatures (Figure 8, Figure 9 & Figure 10). Among all these plots Figure 10 yielded a very high correlation at all temperatures under investigation. Moreover, the plotted lines passed through the zero point.
Both the conventional integral approach and differential approach were used to evaluate the activation energy of the fusion process.
In the integral approach the relationship between the rate constant k and temperature is given by the Arrhenius equation
where A is the frequency factor and E is the apparent activation energy. Apparent activation energy determined from the Arrhenius type plots (Figure 11), where - lnK. Versus 1/T is plotted for F1 model. Slope of the plot gave E/R and activation energy found to be 6.452kJ/mol.
In the differential approach activation energy was determined in three different extraction levels (α) i.e. α = 0.3, 0.4 and 0.5 of alumina by differential approach. Time of attaining different extraction level at different temperatures are cross plotted in Figure 12. From these figures we get values of activation energy for α = 0.3, 0.4 and 0.5 were 6.63, 6.06 and 6.85kJ/mol respectively.
The optimum conditions for the maximum yield of alumina from dross and the kinetics for the extraction reaction were studied in this work. Several parameters i.e. fusion reagent (NaOH) to dross ratio, temperature of fusion and time of fusion were studied in this study. Maximum extraction of alumina was obtained at NaOH to dross ratio of 3.5 and 750°C at 60 minutes. The rate of alumina extraction followed the Avrami-Erofeev equation: -LN (1-α) = (k3t)m where m=3/2 with apparent activation energy of about 6.452kJ/mol.
The authors are grateful to Bangladesh University of Engineering and Technology (BUET) for providing the funds for this study and to Bangladesh Council of Scientific and Industrial Research (BCSIR)) for providing the necessary facilities for this study and to Dr. Abdul Gafur for his help to perform the analysis.
|||S. Freti, J.D. Bbornand & K. Buxman. “Metallurgy of dross formation on aluminium melts” Light Metal, 1982, AIME, pp. 1003-16.|
|||Aluminium Company of America. D.L. Stewart et al., Salt based melting process Int C. C25C3/06 US 5.057, 194 Oct.15 1991.|
|||Christie, P. and Derry, R., Alumina from indigenous U. K. resources, a review of possibilities, Warren Spring Laboratory, Report No. LR (219) ME, 1976.|
|||Qi-ming Feng, Yun Chen, Yan-hai Shao, Guo-fan Zhang, Le-ming Ou, Yi-ping Lu, “New technique of comprehensive utilization of spent Al2O3-based catalyst”, J. Cent. South Univ. Technol., Vol. 13 No. 2, pp 151-155 April 2006.|
|||Phillips, C V and Wills, K J, A laboratory study of the extraction of alumina of smelter grade from China clay micaceous residues by a nitric acid route, Hydrometallurgy, Vol. 9, pp 15-28, 1982.|
|||Bazin C., El-Quassirri K., Uuellet V., “Sequential leaching for the recovery of alumina from a Canadian clay”, Hydrometallurgy, Vol. 88, pp 196-201, 2007.|
|||Felker K., Seeley F., Egan Z., Kelmers D., “Aluminum from fly ash”, ChemTech, Vol. 12, pp 123, 1982.|
|||Aglietti E.F., Tavani E.L., Lopez J.M. Porto, “Acid process for the extraction of aluminum from argentine weathered basalts”, Minerals Engineering, Vol. 3, No. ¾, pp 331-343, 1990.|
|||Aglietti E.F., Tavani E.L., Tedesco P.H., Lopez J.M. Porto, “Alumina extraction from Northeastern Red Soil of Argentina”, Hydrometallurgy, Vol. 17, pp 167-176, 1987.|
|||Amer, A.M., “Extracting Aluminium from Dross Tailing ”, The Journal of The Minerals, Metals & Materials Society, Volume 54, Number 11, 1 November 2002 , pp. 72-75(4).|
|||Miskufova A.,Petranikova, Kovacs M., Briancin J., Havlik T., Orac D., “Leaching of Aluminium Dross in Alkaline Solution”, European Metallurgical Conference, Vol. 4, pp. 1-11, June 28-July 1, 2009, Innsbruck, Austria.|
|||Martin Beaulieu, Stephane Chabot, Yves Charest, Ancienne-Lorette, Jean-Francois Savard, “Processes for Treating Aluminium Dross Residues”, United States Patent 2008/0159935 A1, Publication Jul. 3,2008.|
|||Lucheva B., Tsonev Ts., Petkov R. “Non-waste aluminum recycling”, Journal of the University of Chemical Technology and Metallurgy, 40, 4, 2005, 335-338.|
|||Park, Hyung-Kyu, Lee, Hoo-In, Yoon, Eui-Pak.: Process for recycling waste aluminum dross, United States Patent 6296817, Publication 10/02/2001|
|||Seidel A., Sluszny A., Shelef G., Zimmels Y., “Self inhibition of aluminum leaching from coal fly ash by sulfuric acid [J]”. Chemical Engineering Journal, 1999, 72: 195-207.|